# 90° phase-matched up-conversion of CO_{2} laser radiation in AgGa_{0.86}In_{0.14}S_{2}

- First Online:

- Received:

DOI: 10.1007/s00340-012-5210-7

- Cite this article as:
- Tanno, F. & Kato, K. Appl. Phys. B (2012) 109: 367. doi:10.1007/s00340-012-5210-7

- 299 Downloads

## Abstract

The CO_{2} laser radiation at 10.5910–9.2714 μm was up-converted to the visible in the 90° phase-matched AgGa_{0.86}In_{0.14}S_{2} crystal by mixing with the output of the 0.3547 μm pumped BBO optical parametric oscillator at 25–120 °C. The new Sellmeier and thermo-optic dispersion formulas that reproduce these experimental results correctly as well as the previously published data [Banerjee et al. in Appl Phys B 87:101, (2007); Opt Commun 227:202 (2007)] for difference-frequency generation at 4.05–6.98 μm and second-harmonic generation at 5.2955 μm are presented.

## 1 Introduction

In previous publications [1, 2], we have reported the Sellmeier and thermo-optic dispersion formulas for AgGa_{0.86}In_{0.14}S_{2} that provide a good reproduction for difference-frequency generation (DFG) at 4.05–6.98 μm and second-harmonic generation (SHG) at 5.2955 μm. However, a somewhat large discrepancy between theory and experiment was encountered for the 90° phase-matched up-conversion of the CO_{2} laser radiation achieved in this crystal. For instance, the experimentally observed OPO pump wavelengths for up-conversion of the 10.5910–9.2714 μm radiation are 14–17 nm shorter than the values given by the above-mentioned Sellmeier equations. In addition, a significant difference between theory and experiment was found for the temperature-dependent phase-matching conditions for this process. Thus, we have corrected these formulas so as to satisfy the new experimental results, and simultaneously fit the data points presented in [1, 2].

Here, we report the new experimental results on the 90° phase-matched up-conversion of the CO_{2} laser radiation in AgGa_{0.86}In_{0.14}S_{2} and the new Sellmeier and thermo-optic dispersion formulas for this crystal.

## 2 Experiments and discussions

The experiments were carried out with a step-tunable CW CO_{2} laser and a 0.3547 μm pumped BBO optical parametric oscillator (OPO) as the pump source. Both beams were combined with a ZnSe optical flat and collinearly incident on the refabricated, 7-mm-long, θ = 90° cut AgGa_{0.84}In_{0.16}S_{2} crystal mounted on the temperature controlled oven.

The OPO pump power was adjusted to 5–10 mJ at 10 Hz to avoid the surface damage of the AgGa_{0.84}In_{0.16}S_{2} crystal, and the CO_{2} laser power was adjusted to less than 20 mW to avoid local heating. The unfocused beam diameter was 4 mm for the former and 2 mm for the latter.

The pump and output wavelengths were measured by a 0.5-m spectrometer with an accuracy of less than 0.1 nm.

_{2}laser wavelengths at 9.2714–10.5910 μm, and by tuning the BBO/OPO wavelength from 0.65 to 0.70 μm, we have measured the 90° phase-matching pump wavelengths at 25 °C. The resulting experimental points (open circles) are shown in Fig. 1 together with the theoretical curves (A) and (B) that were calculated with the Sellmeier equations of Banerjee et al. [1, 2] for this crystal and those of Badikov et al. [3] for AgGa

_{1 − x}In

_{x}S

_{2}(

*x*= 0.008 and 0.20), which differ significantly from the data points. The real line (C) is calculated with the following Sellmeier equations:

The measured acceptance angles and spectral phase-matching bandwidths at full-width at half-maximum (FWHM) are Δθ_{int}·ℓ^{½} = (2.3 ± 0.1) deg cm^{½} and Δλ_{p}·ℓ = (0.4 ± 0.1) nm cm, which agree well with the theoretical values of Δθ_{int}·ℓ^{½} = 2.35 deg cm^{½} and Δλ_{p}· ℓ = 0.39 nm cm for the CO_{2} laser wavelength of 10.5910 μm and Δθ_{int}·ℓ^{½} = 2.34 deg cm^{½} and Δλ_{p}·ℓ = 0.48 nm cm for the CO_{2} laser wavelength of 9.2714 μm.

Note that the ordinary and extraordinary refractive indices of AgGa_{1 − x}In_{x}S_{2} increase and the birefringence decrease as a function of In concentrations [3] as in the case of AgGa_{1 − x}In_{x}Se_{2} [4]. While the Sellmeier equations of Banerjee et al. [1, 2] give the ordinary refractive indices that are smaller than those of pure AgGaS_{2} [5] at wavelengths longer than 2.42 μm; in contrast, the new Sellmeier equations give the normal dispersion [*n*(AgGa_{0.86}In_{0.14}S_{2}) > *n*(AgGaS_{2})] throughout the whole spectral range. In addition, this index formula correctly reproduces the 90° phase-matched DFG between the Ti:Al_{2}O_{3} laser at 0.84274 μm and the Nd:YAG laser at 1.0642 μm as well as the phase-matching angle of θ_{PM} = 80.8° and 73.0° for SHG of the CO_{2} laser lines at 10.5910 [1, 2] and 10.2466 μm, respectively.

_{2}laser wavelengths of 10.5910 and 9.5525 μm are shown in Fig. 2.

_{p}/d

*T*= 0.101 and 0.108 nm/ °C for the CO

_{2}laser wavelength of 10.5910 and 9.5525 μm, respectively. The temperature phase-matching bandwidth (FWHM) for this process is Δ

*T*ℓ = (3.4 ± 0.1) °C cm, which agrees well with the calculated values of Δ

*T*ℓ = 3.3 and 3.5 °C cm for the respective CO

_{2}laser wavelengths of 10.5910 and 9.5525 μm.

_{2}laser line at 10.5910 μm given by Banerjee et al. [1, 2]. at 25–203 °C. However, because our calculated values for DFG based on the Nd:YAG laser do not fit their data points shown in Figs. 3 and 4 of [2] except at 120 °C, we have carefully checked these data points and found a distinct difference between the DFG wavelengths obtained at 25 °C by mixing the Ti:Al

_{2}O

_{3}laser the Nd:YAG laser [1] and by mixing the BBO/OPO and Nd:YAG laser [2] in the same crystal. The former is 4.0497 μm as noted in the preceding, while the latter is 4.0258 μm (Fig. 3 of [2]).

In order to clarify this inconsistency, we have once again measured DFG between the BBO/OPO and the Nd:YAG laser under the identical experimental conditions described in [2]. The resulting tuning points (open circles) are shown in Figs. 3 and 4 together with the data points (triangles) taken from [2]. As can be seen from these figures, our data points agree excellently with the theoretical values calculated with Eqs. (1) and (2). Thus, the data point shown in Fig. 3 of [2] is thought to be in error.

## 3 Conclusion

In summary, we have reported the 90° phase-matched up-conversion of the CO_{2} laser radiation at 9.2714–10.5910 μm in AgGa_{0.86}In_{0.14}S_{2}. These data were used to construct the new Sellmeier and thermo-optic dispersion formulas that provide the excellent reproduction of these experimental results as well as the previously published data [1, 2] of DFG at 4.05–6.98 μm and SHG of the CO_{2} laser at 10.5910 μm. We believe that these Sellmeier and thermo-optic dispersion formulas are highly useful for predicting the temperature-dependent phase-matching conditions for frequency conversion in the AgGa_{1−x}In_{x}S_{2} (*x* ≦ 0.14) crystals when combined with our index and thermo-optic dispersion formulas for pure AgGaS_{2} [5].

## Open Access

This article is distributed under the terms of the Creative Commons Attribution License which permits any use, distribution, and reproduction in any medium, provided the original author(s) and the source are credited.